Crystal structure, stability range and hardness of intermetallic phases formed in Al-Fe binary systems at room temperature .
In this chapter, results of our recent investigations on Al-25%Fe (at.%), Al-30%Fe and Al-34.5%Fe alloys close to Al3Fe, Al5Fe2 and Al2Fe intermetallic phases have been discussed. The effect of process parameters on structural aspects and mechanical behaviour of Al-Fe intermetallics has been studied. The high melting intermetallics that are difficult to prepare by conventional processing technique are easily synthesized in nanocrystalline state with a homogeneous structure by mechanical means. In this process, we have come out with a single orthorhombic Al5Fe2 nanocrystalline intermetallic phase. Hardness measurements of intermetallic revealed an increase in hardness with a decreasing grain size up to a critical grain size, followed by a decrease. A decrease in hardness with a grain size refinement, an indication of softening behaviour, demonstrating the Inverse Hall-Petch (IHP)-like phenomenon has been observed in intermetallic compounds. The deviation from the regular Hall-Petch (HP) behaviour has been discussed using various deformation models based on the dislocations and grain boundary-mediated processes. The study is focused on investigations of Al-rich iron aluminide intermetallics to understand the structure property correlations.
- high-energy ball milling
- inverse Hall-Petch
- nanostructured materials
- mechanical properties
- deformation mechanisms
- grain boundary sliding
Intermetallics represent a manifold class of materials that possess intermediate properties between metallic and non-metallic materials. Intermetallic phases and compounds are formed by a combination of two or more metals falling at or near a fixed stoichiometric ratio and exhibit different crystal structure and properties than their constituent elements. The composition of an intermetallic may vary within a restricted composition range known as homogeneity range. Since 2500 BC, metallurgists have used intermetallics, and its phases have attracted significant interests during the last few decades since they offer new prospects for developing structural materials for high-temperature applications.
An increased need for new and novel materials with specified properties and particular application has attracted greater attention of metallurgists and material scientists in recent years. Intermetallics are one such material with a vast potential for application in a wide range of technologically important areas . The first observation of an intermetallic was made in 1839 by Karl Karsten, when he observed a discontinuity in the action of acids on alloys of copper and zinc at the equi-atomic composition and suggested the formation of a compound. The compound is now popularly called as β-brass (CuZn). Intermetallics are already indispensable in many applications and offer the possibility of providing additional breakthrough in performance in, for example, high-temperature structural materials, magnetic materials and hydrogen storage materials. As a by-product of amorphization studies or alloying development, nanocrystalline intermetallic compounds can be synthesized. Nanocrystalline intermetallics possess improved mechanical properties at an ambient temperature. Bohn et al.  have suggested that nanocrystalline intermetallic compounds may have improved mechanical properties. Their study concludes several possible ways of improving strength and ductility. However, the strength of elemental nanocrystalline metals can be increased by factors of 4–5 over conventional grain size materials , strengthening effects in some hard intermetallics that are more modest of the order of 10–20% . The brittle nature of most intermetallics requires powder metallurgical processing route. Amorphization of intermetallic compounds by mechanical alloying (MA) was first reported by Ermakov et al. [5, 6] in Y-Co and Gd-Co systems. Amorphous phases from elemental powder mixtures or powders of intermetallics synthesized by high-energy ball milling have attained an unprecedented interest. A polymorphous phase transformation from crystalline phase to amorphous phase can occur when the free energy of an intermetallic compound is raised by severe mechanical deformation above that of the amorphous phase. The observed transformation could be ascribed to an increased volume fraction of grain boundaries and simultaneous disordering . Zou et al.  reported the formation of amorphous phase in Al-Fe alloy at early stages of MA. It has also been reported that during prolonged milling, amorphous phase undergoes crystallization to form intermetallics.
1.2. Al-Fe intermetallics
Considering all excellent physical and mechanical properties of aluminium, it has become an important element in intermetallics. Iron (Fe) and aluminium (Al) alloys rank among the most important engineering materials because they provide good properties at a low material cost in many applications . Iron aluminide compounds are solid examples of the use of aluminium in intermetallics industry. Changing the aluminium content in iron-aluminium system leads to different iron aluminide compounds. Al-rich iron aluminides are characterized by low density, but also by lower strength and hardness than Fe3Al or FeAl ones. However, the strength and hardness can be improved by grain size refinement, especially to nanometric scale. Having their strength increased, Al-based intermetallics possess a high specific strength. Table 1 indicates the crystal structure, stability range and hardness for the Al-Fe intermetallic phases. Studies on Al-Fe system have been concentrated mainly on mechanical alloying (MA) with individual elements [11, 12, 13, 14]. Moreover, similar structures have been evidenced for a range of Al content. In Al-Fe intermetallic, Al2Fe compound retains the lowest possible symmetry crystal structure, triclinic (Pearson symbol aP19) . Due to its lowest symmetry, the triclinic phase transforms to a high-symmetry Al5Fe2 orthorhombic (Pearson symbol oC24) in the nearby composition. Stability calculations utilizing first principles total energy envisage that oC24 structure has a much lower atomic density than aP19 structure, resulting in a high vibrational entropy and hence aP19 structure loses stability to the oC24 structure at elevated temperatures .
|Vickers hardness (9.8 N)|
1.3. Al-Fe intermetallics by mechanical alloying/mechanical milling
Nanocrystalline intermetallic compounds are said to have enhanced properties as compared to conventional grain-sized materials. MA/mechanical milling (MM) has been considered a suitable processing method capable of attaining this goal of producing nanostructured materials . The synthesis of intermetallics through MA/MM has emerged as a valuable method for the following reasons: (1) the synthesis of intermetallics which are difficult to prepare by conventional methods, (2) to obtain enhanced properties through microstructural modifications and (3) the synthesis of nonequilibrium microstructures, such as amorphous alloys at intermetallic compositions. The formation of amorphous phase in Al-20 at.%Fe alloy was reported by Zhou et al. after 240 h of MA . Almost complete amorphous phase in Al-(17–33) at.%Fe system was observed by Huang et al. . In a similar study, for Al-34 at.%Fe, Al-25 at.%Fe, Al-25 at.%Fe and Al-20 at.%Fe system, respectively, crystalline phases were evidenced by Enzo et al. and Cardellini et al. [19, 20]. For a composition range of Al-34.7–35.3 at.%Fe intermetallic phase, Al5Fe2 along with Al2Fe was observed by Gasior et al. . A comparison of the phases formed in Al-Fe alloys as analysed from the X-ray diffraction (XRD) traces is given in Table 2. In addition to MA experiments, Romero et al.  reported the effect of mechanical milling (MM) on the structural evolution of as-cast Al2Fe and Al5Fe2 intermetallic systems at different short milling times. Apart from this study, no other reports on systematic investigation on the structural evolution of as-cast Al-rich iron aluminide intermetallics are available. The possibility of nanostructured and amorphous phases and their stability by MM can be explored from the thermodynamic explanation based on a semi-experimental theory of improved Miedema’s model (Zhang model)  by calculating the Gibbs free energy of the phases from their enthalpy of formation.
|Al-34.7–35.3 at.%Fe||Al5Fe2 + Al2Fe||Gasior et al. |
|Al-28.45 at.%Fe||Al5Fe2 + Al2Fe||Romero et al. |
|Al-25 at.%Fe||Al5Fe2||Cardellini et al. |
|Al-20 at.%Fe||Amorphous||Zhou et al. |
|Al-20 at.%Fe||Al5Fe2||Cardellini et al. |
|Al-34 at.%Fe||α-Al||Enzo et al. |
|Al-17–33 at.%Fe||Amorphous||Huang et al. |
|Al-25 at.%Fe||α-Al||Enzo et al. |
|Al-33.28 at.%Fe||Al5Fe2 + Al2Fe||Romero et al. |
1.4. Nanostructured materials
Nanostructured materials are an important class of metastable materials that are produced by ball milling. Materials are considered as nanostructured if the crystallite size is of the order of few nanometres (typically 1–100 nm). A novel way of transforming a material to a metastable state is to reduce its grain size from micrometres to nanometres, when the proportion of atoms at the grain boundaries is equal to or higher than those inside the grains. The fine grain-sized materials are structurally characterized by a large volume fraction of atoms in or near the grain boundaries, which significantly alter the material properties that are often superior or sometimes completely new in comparison with conventional coarse-grained polycrystalline materials. In 1987, Thompson and Politis first reported the formation of a nanostructured material synthesized by MA . A mechanism for the formation of nanostructures by MA/MM has been reported . In 1992, Li et al. proposed a relation between grain size and the time of milling by a model for the refinement of grain size during ball milling .
It is given by
The balance between defect/dislocation structure introduced by the plastic deformation of milling and its recovery processes forms the main criteria to decide on the minimum grain size that can be achieved by mechanical milling. This process will result in a lower bound for the grain size of pure metals and alloys and reveals that a small grain size itself provides a limit for further grain refinement on milling. On the whole, when the material exhibits a nanocrystalline structure, hence microstructural refinement cannot be observed and further deformation can only be accomplished by grain boundary sliding (GBS). It has been suggested that the minimum grain size that can be achieved by milling is determined by the balance between defect/dislocation structure introduced by the plastic deformation of milling and its recovery by thermal processes. This contributes to a lower bound for the grain size of pure metals and alloys and reveals that a small grain size itself provides a limit for further grain refinement on milling. Once the whole material exhibits a nanocrystalline structure, further deformation can only be accomplished by grain boundary sliding, and hence microstructural refinement cannot be observed. The limiting grain size is normally determined by the minimum grain size that can sustain a dislocation pile-up within a grain and by the rate of recovery . Earlier researchers have proposed that hardness decreases at small grain sizes as it becomes impossible to accommodate the high density of dislocations required to form a pile-up at a grain boundary [28, 29].
2. Effect of process parameters on mechanical properties
Despite the same composition of initial powder mixture, various structures can evolve depending on the parameters of the milling process. In this section, the effect of mechanical milling (MM) on the structural evolution of as-cast Al-rich iron aluminide intermetallics through different stages of milling and its mechanical behaviour has been discussed. The mechanical properties of intermetallics are closely related to their structure and its stability . Grain boundaries are the most important microstructural elements of materials, and their strengthening effect is phenomenologically quantified by a classical HP relationship. However, deviations from HP relation contributing to a softening behaviour are also observed after a critical grain size (dc). Due to the difference in the mechanical properties, which is greatly influenced by the microstructure [31, 32] of the intermetallic phases and its transformation during milling, a significant difference in the force displacement curves manifested not only by the shapes of the load-penetration depth but also by the maximum penetration depth attained under the same conditions was observed when evaluated using Oliver and Pharr method  (Oliver et al. (2004)). For intermetallics that are concerned, the effort has been directed mainly towards the development of high strength materials, and reports that address softening behaviour in nanoscale microstructures or composite microstructures are very rare. Al-25 at.%Fe, Al-30 at.%Fe and Al-34.5 at.% Fe close to Al3Fe, Al5Fe2 and Al2Fe intermetallic phases have been prepared in an arc-melting furnace under argon atmosphere. The pre-alloyed ingots were brittle and therefore repeatedly crushed and mechanically sieved to powders. Mechanical milling of the crushed powders was then carried out using high-energy planetary ball mill. This study provides some insights to understand the correlation between the process parameters and the mechanical behaviour of Al-Fe intermetallics.
2.1. Microstructural and structural features
Figure 1 shows X-ray diffraction pattern of crushed as-cast powders of Al-25 at.%Fe alloy. Diffraction peaks confirm mostly single-phase complex monoclinic Al3Fe (θ) structure. Figure 2 shows the structural evolution of Al3Fe intermetallic subjected to varying hours of MM. A relatively broad peak was observed because of the fine crystallite size and the presence of strain in the powder at early stages of milling. After 10–20 h of milling, the formation of η-Al5Fe2 was evidenced as an intermediate phase. The presence of η-Al5Fe2 prevailed till 30 h of milling, but a further increase in the milling time led to the broadening of these peaks too. The intermetallic Al3Fe phase was completely transformed into the amorphous state after 50 h of milling. A broad halo at 2θ = 40–47o suggests that the formation of an amorphous phase was seen from the XRD patterns shown in Figure 2. Eventually, the phase transformations during MM for Al–25 at.%Fe alloy powders are expressed as follows:
Transmission electron microscope (TEM) image of Al-25 at.%Fe alloy milled for 50 h is shown in Figure 3. The micrograph showed the co-existence of nanocrystalline, η-Al5Fe2 and amorphous phases, and a diffuse ring along with diffraction spots was evidenced in a selected area diffraction (SAD) pattern. However, complete amorphization after 50 h of milling was observed in its corresponding XRD pattern. The broadening of the peak observed in XRD corresponds not only to the formation of amorphous structure but also to the refinement of the nanocrystalline structure induced by mechanical milling, and hence residual crystalline phase is present along with amorphous phase. The characteristic X-ray diffraction pattern of as-cast powders of Al-30 at.% Fe alloy is shown in Figure 4. The most intense diffraction peaks (2 2 1) and (3 1 1) at 2 = 42.55 and 43.79 were found in the as-cast alloy. JCPDS data suggest that this compound is representative of a single Al5Fe2 orthorhombic phase (JCPDS reference code: 00-047-1435)  with lattice parameters of a = 0.7648 nm, b = 0.6413 nm and c = 0.4216 nm. Results of XRD patterns showing the structural evolution of Al5Fe2 intermetallic subjected to MM for different ranges of milling time are shown in Figure 5. It is apparent that milling up to 30-h disappearance of all peaks except for major peaks of (2 2 1) and (3 1 1) was observed. The broadening observed in the diffraction peak can be attributed to the major peaks overlapping from the intermetallic phase. The results obtained are in contrary to Al5Fe2 obtained by MA route , where complete formation of intermetallic phase was achieved in Al-25%Fe after 30 h of MA, and the formation of amorphous phase was seen after 50 h of MA. Further in a similar work, Hunag et al.  observed the formation of the Al5Fe2 intermetallic in Al-24.4%Fe powder heat-treated at 500°C after MA for 180 h. It is interesting to note that the XRD peaks undergo broadening in the course of mechanical milling up to 50 h mainly due to cumulative effects of grain refinement and lattice strain. A bright field and dark-filed image of 50 h-milled Al-30 at.% Fe alloy (Figure 6a and b) reveals the presence of a nanocrystalline structure suggesting the presence of a nanostructured Al5Fe2 intermetallic phase which agrees well with the structural evolution observed from the XRD pattern.
Figure 7 shows the XRD pattern of as-cast Al-34.5 at.%Fe alloy. Diffraction peak confirms a mixture of intermetallic phases namely ζ-Al2Fe and η-Al5Fe2. For a compositional range of 34.7–35.3 at.%Fe in Al alloy, the observed intermetallic phase Al5Fe2 along with Al2Fe was observed by Gasior et al. . Phase transformation from crystalline triclinic Al2Fe and orthorhombic Al5Fe2 to the partial formation of amorphous phase at 10 h of MM resulted in Al-34.5 at.%Fe alloy. Due to the peak overlapping from the mixture of intermetallic phases, a width was observed in the most, intense diffraction peak. With continued milling, a decrease in the width of Bragg peaks and an increase in peak resolution were noted, indicating that Al2Fe intermetallic phase becomes unstable as a result of MM. The detected phase transition that occurred during milling process is suggestive of the accumulation of structural defects which increases the stored energy in the intermetallic material.
As evidenced in Figure 7, complete amorphization after 40 h of milling was achieved in this particular composition with prolonged milling time. The fine grain size and consequently large surface area induced by MM make the powders of this particular composition pyrophoric in nature after 40 h of milling. The same was observed even when milling experiments were paused periodically at regular intervals of every 30 min. Phase transformations achieved as a result of MM for Al-34.5 at.%Fe alloy powders are expressed as.
The orthorhombic structure of Al5Fe2 phase features a rigid framework of fully occupied Al and Fe sites as well as partially occupied Al sites confined within channels . This kind of structure makes it unstable when subjected to a severe plastic deformation leading to an amorphous phase. Further, for the present milling conditions, Al5Fe2 phase was also found to be stable with respect to its competing phases. Due to lattice defects introduced by MM which promote spontaneous transformation to the amorphous phase, the intermetallic compounds with narrow homogeneity ranges tend to become amorphous . A high-resolution TEM micrograph corresponding to Al-34.5 at.%Fe alloy milled for 40 h is shown in Figure 8. The micrograph reveals a single amorphous phase and is corroborated by the fast Fourier transformation-selected area diffraction (FFT-SAD) pattern.
Differential thermal analysis (DTA) trace of 50 h-milled Al-25 at.%Fe intermetallic powders is shown in Figure 9a. Upon heating the as-milled powders at a constant rate of 10°C/min, one exothermic peak at around 1090°C was revealed. An equilibrium diagram of Al-Fe  confirms that this peak corresponds to the melting point of the Al5Fe2 intermetallic phase, formed as a result of phase transformation of monoclinic Al3Fe after high-energy ball milling. DTA curves of as-cast Al-34.5 at.%Fe alloy and ball-milled powder obtained after 40 h of milling are shown in Figure 9b. As marked by arrows, the thermal curves indicated the presence of two endothermic peaks for the as-cast alloy. According to the equilibrium phase diagram, the first peak at 1090°C corresponds to the melting point of Al5Fe2 intermetallic compound, and the second peak at a higher temperature (1149°C) as marked by an arrow is due to the melting of Al2Fe. A single exothermic peak around 1090°C corresponding to Al5Fe2 phase formed as a result of transformation of an Al2Fe intermetallic phase to a high-symmetry phase Al5Fe2 after high-energy milling was evidenced from DTA trace of 40 h milled powders. Thermal analysis results agree well with the XRD results as shown in Figure 7, where the pattern corresponds to both Al5Fe2 and Al2Fe phases for as-cast alloy and a single Al5Fe2 phase for 40 h milled powders. The calculation of free energy of equilibrium phases was carried out based on the improved Miedema’s model (Zhang model). Table 3 gives the data of Al and Fe necessary for the calculation of Gibbs free energy. The variation of
(for amorphous, two intermetallic compounds and crystalline solid solutions) as a function of composition for different values of
|Element||n1/3 (cm−1)||Φ (V)||K (GPa)||Tm (K)||V2/3 (cm2)||γ (erg/cm2)||ΔHf (kJ/mole)|
2.2. Mechanical properties
Figure 11a shows the milling time dependence of Vickers hardness for Al-25 at.%Fe alloy for various milled powders. The hardness increases with an increase in the milling time and reaches its maximum value between 20 and 30 h of milling and then decreased. A higher hardness value of about 8.6 GPa resulted at 30 h of milling. Thus, the optimum milling time for the studied composition is 30 h. The formation of intermetallic phase, η-Al5Fe2, and its co-existence with amorphous phase could be the reason for the observed peak in hardness values. However, for Al-20 at.%Fe alloy, the microhardness of 12.4 GPa was reported for 20 h of MA followed by cold consolidation and subsequent annealing at 673 K for 2 h . Figure 11b shows the change in microhardness as a function of reciprocal square root of the grain size. It is evident that up to a grain size of about 42 nm, the values of hardness increase linearly with the reciprocal square root of the grain size. Over the range of grain sizes from 132 to 42 nm, the Hall-Petch (HP) behaviour is established. Further, the HP slope, which describes grain size sensitivity, also have a similar value to that found for conventional grain sizes. This behaviour is ascribed to the refinement in the grain size produced as a result of MM. However, it is worth noting that when the crystallite sizes drop below 42 nm, the slope of the Hall-Petch plot becomes negative. The evidenced effect could be due to a softening behaviour, an attribute described as an inverse H-P phenomenon [28, 29]. Theoretically, the critical value of the grain size below which the plot becomes negative can be calculated from Eq. (4)
To examine the discrepancy involved in a dislocation pile-up mechanism related to a softening behaviour, the critical grain size was calculated and found that the theoretical value obtained was about 8 nm in comparison to the experimental value of 42 nm. It can be concluded that the presence of competing/contributing effects of nanocrystalline and amorphous phase could be the reason for the differences observed. Though the critical grain size for nanocrystalline materials where softening occurs can be predicted by a dislocation pile-up model, it fails for composite structure involving nanocrystalline and amorphous phase. Figure 12 shows the microhardness variation with a milling time for Al-30 at.% Fe alloy. It is apparent from the plot that a single Al5Fe2 intermetallic phase subjected to MM resulted in Hall-Petch (HP) break-down and showed two distinct behaviours. The break-down of Hall-Petch for the averaged hardness can be attributed to the deformation mechanism and structure that occur due to mechanical milling. The HP slope decreases below a critical grain size and becomes negative, indicating an inverse Hall-Petch (IHP) behaviour. The HP strengthening has been ascribed to the pile-up of dislocations and their resistance to slip transfer. However, HP behaviour for grain size ranging from 101 to 32 nm and an IHP behaviour for grain sizes less than 32 nm was observed. The variation of microhardness as a function of milling time for Al-34.5 at.%Fe alloy is shown in Figure 13. The figure clearly demonstrates that the hardness of the alloy increased with increasing the milling time at the early stage and after prolonged milling reveals softening during the formation of amorphous phase. The hardness values increase with an increase in the milling time, which is an indicative of the formation of amorphous phase along with crystalline intermetallic phase. A softening behaviour observed at higher milling durations can be attributed to the high volume fraction of grain boundaries resulting in an increased triple junction leading to a grain boundary sliding . The transition from hardening to softening behaviours that occurs in an amorphous phase could be ascribed to mechanisms such as a decrease in the interfacial excess volume and free volume model . However, detailed investigation regarding this issue is needed to understand the softening behaviour. The typical load-displacement curves showing elastic-plastic material response for intermetallic phases milled for various durations, for indentations made to peak loads of 20 mN at room temperature, are presented in Figure 14a and b. Under the same conditions, the force displacement curves showed significant differences manifested not only by the shapes of the load-penetration depth but also by the maximum penetration depth attained. The microstructure of the intermetallic phases and its transformation during milling causes difference in the mechanical properties [29, 40] as evidenced in curves. The standard procedure according to Oliver and Pharr  (Oliver et al. (2004)) was employed to calculate the elastic modulus and hardness values. These parameters, estimated from the curve, are given in Table 4. The evolution of elastic modulus with a milling time indicates a relative complex effect of the phase formation/transformation in Al-Fe alloys.
|Material||Hardness (GPa)||Elastic modulus (GPa)|
|Milling time (h)|
The interatomic distance and the bonding strength between atoms, which is a representation of elastic modulus, are greatly influenced by the severe plastic deformation induced by mechanical milling. The increased hardness and elastic modulus resulted at the early stages of milling are due to the refinement in grain size which resists grain boundary motion. The maximum elastic modulus of 168 and 157 GPa and the peak hardness of about 9.3 and 8.8 GPa at 20 h were observed for Al-25 at.%Fe and Al-34.5 at.%Fe alloys, respectively. After a longer milling time where amorphous phase formation was evidenced, the hardness and elastic modulus values decreased to a factor of about two. The differences in the average values of 0.6 GPa between microhardness and nanohardness observed were ascribed to indentation size effect (ISE) .
3. Effect of grain size on mechanical properties
Mechanical property is an important consideration for the application of materials and depends fundamentally upon their microstructure on a variety of length scales and the nature of bonding among their constituent atoms. Mechanical deformation can be either elastic or plastic. Elastic deformation is effected through reversible changes in the interatomic spacing or the bending and stretching of bonds between atoms; it is governed by the elastic constants or moduli of a material. For metals, such deformation is in general relatively easy owing to the non-local nature of metallic bonding, but for materials with a strong covalent or ionic bonding such as intermetallic compounds, it is difficult. Mechanical properties of nanocrystalline materials display an increasing interest. Reducing the grain sizes not only creates a big impact on the microstructures of the nanocrystalline materials but also alters their mechanical properties significantly. The most important mechanical properties of nanocrystalline metals and alloys include significantly increased hardness, strength and ductility, and so on with respect to the decreasing grain sizes . The mechanical properties of NC materials not only depend on the average grain size but also depend on the grain size distribution and the microstructure, such as the grain boundary structures have a critical effect on their mechanical properties.
3.1. Inverse Hall-Petch effect in nanocrystalline materials
As suggested by the well-known Hall-Petch relationship, the mechanical properties of the material increase with the inverse square root of the grain size. However, as the grain size decreases to the submicrometre range, the
3.2. Deformation mechanisms
The expansion of the understanding of deformation of conventional polycrystalline materials to materials with grain sizes on the scale of nanometre is, at present, an evolving process. The experimental finding on inverse Hall-Petch has prompted various researches to propose models pertaining to their mechanism of deformation. Of the proposed models, different deformation mechanisms for nanocrystalline Al5Fe2 intermetallic are discussed subsequently.
3.2.1. Dislocation pile-up model
It is pertinent to point out that dislocation activities  have been shown to exist in some nanocrystalline materials. Nevertheless, the dislocation activity can be considered virtually absent in nanostructured materials where the grain size is lower than the minimum required distance to be maintained between the two dislocations. Therefore, the HP relation is expected to witness a transition below a critical grain size, . TEM and molecular dynamics (MD) simulation have also demonstrated that the grain boundaries can act as a source and a sink for dislocations. In nanomaterials, Hall-Petch behaviour breaks down because the grain is too small for dislocations to pile-up. In a polycrystalline sample, each individual grain will no longer be able to support more than one dislocation . Using the concept proposed by Nieh and Wadsworth, Farghalli and co-workers [47, 48] developed a relationship between the critical grain size and hardness for the critical grain size below which softening occurs. Assuming that the stress field of a dislocation is valid at the nanoscale, and on the suggestion that fine grain sizes affect dislocation self-energy, a mathematical analysis was proposed and it leads to Eq. (5):
is the Burgers vector,
the measured hardness,
the hardness equivalent of the applied stress at the moment of load application,
the shear modulus and
is a constant ranging equals 0.6 . By using the material parameters for Al5Fe2 (
3.2.2. Grain boundary shearing/sliding model
It is clearly evident that the models based on dislocation pile-up could not account for grain size softening. For such fine grains, the deformation based on dislocation mechanisms becomes less dominant, and the mode of deformation based on grain boundary phase (via grain boundary shearing) comes into picture . This would lead to a decrease in hardness and strength, since strain hardening due to dislocation will be absent and the grain boundary will be softer . The deformation in nanocrystalline materials below a critical grain size has been analysed as a thermally activated process, determining the parameters such as activation energy (∆F) and activation volume (∆V). Conrad and Narayan  considered the thermally activated deformation and proposed a rate-controlling equation, which is given as
The parameters in Eq. (6) are the Debye frequency,
(1013 s−1); the grain boundary width taken to be 3
the atomic diameter; the effective stress,
is the applied stress and
is the threshold stress;
, the activation volume taken to be
the Helmholtz free energy;
The model was validated for IHP regime of the current experimental data, and the experimentally observed and calculated hardness values of this system are shown in Figure 15. The degree of fit, as described by coefficient of correlation, for all the three expressions Hv versus ln(L), Hv versus L (these two describe the rigorous and approximate forms of the relationship in the model by Conrad and Narayan ) and Hv versus (L-L0)0.5/L , is very similar, and the findings are presented in Table 5. On this basis, both the models are acceptable. The preceding discussion shows that although the model proposed by Conard and Narayan explains the IHP effect, the parameters used for validation is quite unreasonable: (1) the effective stress is taken to be equal to the applied stress, that is, the strain-rate sensitivity index, m = 1.0. However, in nanocrystalline materials at room temperature, the value of m is in the range of 0.02–0.08 [54, 55] and (2) further, the strain rate was assumed as 10−3 s−1, but according to [56, 57], the strain rate lies in the range of 5 × 10−2 to 5 × 10−4 s−1. Thus, the experimental data were analysed using both the strain rate values and the free energy of activation,
for the rate-controlling process (mesoscopic GBS), and refined values of
were determined as a function of strain rate and the results are presented in Table 6. The following observations are interesting: the relative change in hardness as one goes from the HP to the IHP region is much less in intermetallics than in nanocrystalline materials. This aspect needs further study. However, it is clear that the observed IHP effect in intermetallics also could be explained in terms of the mesoscopic grain boundary sliding controlled flow process, as with the other classes of materials. Finally, as the value of N for the system (Table 6) is less than one, it follows from the model [58, 59, 60] that the plane interface formation in these intermetallics of the studied grain size ranges is the result of dislocations/partial dislocations being emitted from the deforming boundary, which then traverse the grain and get absorbed at the opposite boundary [58, 59]. The value of
equals 70 kJ/mol and
equals (1.887 × 10−10)3 nm3 was obtained by plotting experimental hardness against ln d. A plot of
for the IHP data is presented in Figure 16. In addition,
values obtained by linear fit of both experimental hardness values against
|System||L, nm||H, GPa||Correlation coefficient of H and|
|System||N||L, nm||τo, GPa||, refined*|
In this section, the recent progress in the synthesis of Al-Fe intermetallics and their softening behaviour using various deformation mechanisms is discussed. In this process, Al-25 at.%Fe and Al-34.5 at.%Fe alloys resulted in Al3Fe and Al2Fe intermetallic phases after normal casting and annealing routes. Monoclinic Al3Fe and triclinic Al2Fe phase was found to be unstable under high-energy milling condition and transformed to orthorhombic Al5Fe2 phase. Nanocrystalline and amorphous phase co-exist for 30 h of milling where the maximum hardness was observed. A microhardness of Al-25 at.%Fe alloy showed strengthening down to a grain size of 42 nm, and Hall-Petch behaviour was thus established over the range of grain sizes from 132 to 42 nm. At the smallest grain size (33 nm), the slope of HP plot becomes negative indicating IHP behaviour.
In addition, Al5Fe2 resulted from Al-30%Fe alloy resulting in the formation of nanocrystalline intermetallic and was found to be quite stable under the present experimental conditions, and the crystallite size of it decreases up to 10 nm with an increase in the milling time. Microhardness measurements of single Al5Fe2 nanocrystalline intermetallic phase produced by mechanical milling resulted in Hall-Petch (HP) break-down and showed two distinct behaviours. The break-down of HP for the averaged microhardness measurements was found to be due to the transition of deformation mechanism from dislocation activity to grain boundary sliding. Dislocation models could not intend the critical grain size at which the HP relation breaks down, and so models based on grain boundaries were considered. Detailed analysis showed that models based on grain boundaries namely grain boundary sliding and thermally activated grain boundary shearing seem to be reasonable in explaining the IHP effect. Grain boundary sliding is ascribed to be a viable deformation mechanism resulting in a softening behaviour observed in this system.
The authors are thankful to Dr. V.C. Srivastava and Prof. K.A. Padmanabhan for many stimulating discussions. One of the authors (Raviathul Basariya) gratefully acknowledges the financial support by L.S. Ameer Dheen, Chennai, India, in the form of Research Fellowship. Sections 2 and 3 of this chapter are reproduced with permission from References [34, 35] (©2015, 2016 Elsevier).
Darolia R. NiAl alloys for high temperature structure applications. The Journal of The Minerals, Metals & Materials Society. 1991; 43(3):44
Bohn R, Hanbold T, Birringer R, Gleiter H. Nanocrystalline intermetallic compounds-an approach to ductility? Scripta Metallurgica et Materialia. 1991; 25:81
Jang JS, Koch CC. The Hall-Petch relationship in nanocrystalline iron produced by ball milling. Scripta Metallurgica et Materialia. 1990; 24:1599
Koch CC, Cho YS. Nanocrystals by high energy ball milling. Nanostructured Materials. 1992; 1:207
Ermakov A, Yurchikov E, Barinov V. The magnetic properties of amorphous Y-Co alloy powders obtained by mechanical comminution. Physics of Metals and Metallography. 1981; 52:50
Yermakov AY, Yurchikov YY, Barinov VA. Magnetic properties of amorphous powders prepared by the mechanical grinding of Y-Co alloys. Fizika Metallov I Metallovedenie. 1981; 52:1184
Koch CC, Whittenberger JD. Review: Mechanical milling/alloying of intermetallics. Intermetallics. 1996; 4:339
Zou Y, Saji S, Kusabiraki T. Fast amorphization and crystallization in Al-Fe binary system by high-energy ball milling. Materials Research Bulletin. 2002; 37:123
Ashby MF. Materials Selection in Mechanical Design. Butterworth-Heinemann: Burlington, MA; 2005
Massalski TB. Binary Phase Diagram. OH, USA: American Society for Metals, Metals Park; 1986: 1 & 2
Mukhopadhyay DK, Suryanarayana C, Froes FH. Structural evolution in mechanically alloyed Al-Fe powders. Metallurgical and Materials Transactions. 1995; 26A:1939
Krasnowski M, Kulik T. Nanocrystalline Al–Fe intermetallics—Lightweight alloys with high hardness. Intermetallics. 2010; 18:47
Mhadhbi M, Khitouni M, Escoda L, Sunol JJ, Dammak M. Microstructure evolution and mechanical properties of nanocrystalline FeAl obtained by mechanical alloying and cold consolidation. Journal of Alloys and Compounds. 2011; 509:3293
Krasnowski M, Kulik T. Nanocrystalline and amorphous Al–Fe alloys containing 60-85% of Al synthesised by mechanical alloying and phase transformations induced by heating of milling products. Materials Chemistry and Physics. 2009; 116:631
Corby RN, Black PJ. The structure of FeAl2 by anomalous dispersion methods. Acta Crystallographica B. 1973; 29:2669
Mihalkovic M, Wisdom M. Structure and stability of Al2Fe and Al5Fe2: First principles total energy and phonon calculations. Physical Review B. 2012; 85:014113
Zhou F, Luck R, Scheffer M, Lang D, Lu K. The crystallization process of amorphous Al80Fe20 alloy powders prepared by ball milling. Journal of Non-Crystalline Solids. 1999; 250-25:704
Huang B, Ishihara KN, Shingu PH. Metastable phases of Al–Fe system by mechanical alloying. Materials Science and Engineering: A. 1997; 231:72
Enzo S, Mulas G, Frattini R. The structure of mechanically alloyed AlxFe(1-x) end-products after annealing. Materials Science Forum. 1998; 269-272:385
Cardellini F, Contini V, Gupta R, Mazzone G, Montone A, Perin A, Principi G. Microstructural evolution of Al–Fe powder mixtures during high energy ball milling. Journal of Materials Science. 1998; 33:2519
Gasior W, Debski A, Moser Z. Formation enthalpy of intermetallic phases from Al-Fe system measured with solution calorimetric method. Intermetallics. 2012; 24:99
Romero-Romero JR, Luis Lopez-Miranda J, Esparza R, Espinosa-Medina MA, Rosas G. High-energy ball-milling of FeAl2 and Fe2Al5 intermetallic systems. Materials Science Forum. 2013; 755:47
Zhang RF, Liu BX. Proposed model for calculating the standard formation enthalpy of binary transition-metal systems. Applied Physics Letters. 2002; 81:1219
Thompson JR, Politis C. Formation of amorphous Ti-Pd Alloys by mechanical alloying methods. Europhysics Letters. 1987; 3:199
Hellstern E, Fecht HJ, Garland C, Johnson WL. Multicomponent ultrafine microstructure. Materials Research Society. 1989; 132:137
Li S, Wang K, Sun L, Wang Z. A simple model for the refinement of nanocrystalline grain size during ball milling. Scripta Metallurgica et Materialia. 1992; 27:437
Eckert J, Holzer JC, Kill CE III, Johnson WL. Structural and thermodynamic properties of nanocrystalline fcc metals prepared by mechanical attrition. Journal of Materials Research. 1992; 7:1751
Padmanabhan KA, Dinda GP, Hahn H, Gleiter H. Inverse Hall-Petch and grain boundary sliding controlled flow in nanocrystalline materials. Materials science and Engineering: A. 2007; 452-453:462
Conrad H, Narayan J. On the grain size softening in nanocrystalline materials. Scripta Materialia. 2000; 42:1025
Zhu J, Miao Y, Guo JT. The effect of boron on charge density distribution in Ni3Al. Acta Materialia. 1997; 45:1989
Xu S, Prasitthipayaong A, Pickel AD, Habib AH, McHenry ME. Mechanical properties of FeCo magnetic particles–based Sn-Ag-Cu solder composites. Applied Physics Letters. 2013; 102:251909
Chromik RR, Vinci RP, Allen SL, Notis MR. Nanoindentation measurements on Cu-Sn and Ag-Sn intermetallic formed in Pb-free solder joints. Journal of Materials Research. 2003; 18:2251
Oliver WC, Pharr GM. Measurement of hardness and elastic modulus by instrumented indentation: Advances in understanding and refinements to methodology. Journal of Materials Research. 2004; 19:3
Raviathul Basariya M, Roy RK, Pramanick AK, Srivastava VC, Mukhopadhyay NK. Structural transition and softening in Al-Fe intermetallic compounds induced by high energy ball milling. Materials Science and Engineering: A. 2015; 638:282
Raviathul Basariya M, Srivastava VC, Mukhopadhyay NK. Inverse Hall-Petch like behaviour in a mechanically milled nanocrystalline Al5Fe2 intermetallic phase. Philosophical Magazine. 2016; 96:2445
Burkhardt U, Yu G, Ellner M, Peters K. Structure refinement of the iron-aluminium phase with the approximate composition Fe2Al5. Acta Crystallographica. 1994;B50:313
Gu N, Henley CL, Mihalkovic M. Co-rich decagonal Al-co-Ni: Predicting structure, orientation order and puckering. Philosophical Magazine. 2006; 86:593
Schwarz RB, Petrich RR, Saw CK. The synthesis of amorphous Ni-Ti alloy powders by mechanical alloying. Journal of Non-Crystalline Solids. 1985; 76:281
Nayak SS, Wollgarten M, Banhart J, Pabi SK, Murty BS. Nanocomposites and an extremely hard nanocrystalline intermetallic of Al-Fe alloys prepared by mechanical alloying. Materials Science Engineering: A. 2010; 527:2370
Carlton CE, Ferreira PJ. What is behind the inverse hall-Petch effect in nanocrystalline materials? Acta Materialia. 2007; 55:3749
Mukhopadhyay NK, Paufler P. Micro- and nanoindentation techniques for mechanical characterization of materials. International Materials Reviews. 2006; 51:209
Siegel RW, Fougere GE. Mechanical properties of nanophase metals. Nanostructured Materials. 1995; 6:205
Chokshi AH, Rosen A, Karch J, Gleiter H. On the validity of the Hall-petch relationship in nanocrystalline materials. Scripta Metallurgica. 1989; 23:1679
Koch CC, Narayan J. The inverse Hall-Petch effect—fact or artifact. Materials Research Society Symposia Proceedings. 2001; 634:B5.1.1
Koch CC. Optimization of strength and ductility in nanocrystalline and ultrafine grained metals. Scripta Materialia. 2003; 49:657
Froseth AG, Derlet PM, Van Swygenhoven H. Dislocations emitted from nanocrystalline grain boundaries: Nucleation and splitting distance. Acta Materialia. 2004; 52:5863
Mohamed FA, Yuwei Xun. Correlations between the minimum grain size produced by milling and material parameters. Materials Science and Engineering R: Reports. 2003; 354:133
Nieh TG, Wadsworth. Hall Petch relation in nanocrystalline solids. Scripta Metallurgica et Materialia. 1991; 25:955
Hirose S, Itoh T, Makita M, Fujii S, Arai S, Sasaki K, Saka H. Defect structure of deformed Fe2Al5 intermetallic compound. Intermetallics. 2003; 11:633
Weertman JR, Averback RS. Mechanical properties. In: Edelstein AS, Cammarata RC, editors. Nanocrystalline Materials: Synthesis, Properties and Applications. Bristol: Institute of Metals Publishing; 1996: 13
Padmanabhan KA, Sripathi S, Hahn H, Gleiter H. Inverse Hall–Petch effect in quasi-and nanocrystalline materials. Materials Letters. 2014; 133:151
Jiang B, Weng GJ. A composite model for the grain-size dependence of yield stress of nanograined materials. Metallurgical and Materials Transactions A: Physical Metallurgy and Materials Science. 2003; 34:765
Raviathul Basariya M, Mukhopadhyay NK, Sripathi S, Padmanabhan KA. Grain size softening effect in intermetallics. Journal of Alloys and Compounds. 2016; 673:199
Padmanabhan KA. Mechanical properties of nanostructured materials. Materials Science and Engineering A. 2001; 304:200
Varam S, Rajulapati KV, BhanuSankaraRao K. Strain rate sensitivity studies on bulk nanocrystalline aluminium by nanoindentation. Journal of Alloys and Compounds. 2014; 585:795
Maier V, Durst K, Mueller J, Backes B, Hoppel HW, Goken M. Nanoindentation strainrate jump tests for determining the local strain-rate sensitivity in nanocrystalline Ni and ultrafine-grained Al. Journal of Materials Research. 2011; 26:1421
Padmanabhan KA, Schlipf J. Model for grain boundary sliding and its relevance to optimal structural superplasticity: Part 1 e theory. Materials Science and Technology. 1996; 12:391
Padmanabhan KA, Gleiter H. Optimal structural superplasticity in metals and ceramics of microcrystalline- and nanocrystalline-grain sizes. Materials Science and Engineering A. 2004; 381:28
Venkatesh TA, Bhattacharya SS, Padmanabhan KA, Schlipf J. Model for grain boundary sliding and its relevance to optimal structural superplasticity. Materials Science and Technology. 1996; 12:635
Ali MNK, Scudino S, Samadi Khoshkhoo M, Stoica M, Srivastava VC, Uhlenwinkel V, Vaughan G, Suryanarayana C, Eckert J. Grain size softening effect in Al62.5Cu25Fe12.5 nanoquasicrystals. Applied Physics Letters. 2013; 103:201914